nano/mesoporous carbon from rice starch for voltammetric · pdf file molecules article...
Post on 06-Sep-2020
Embed Size (px)
Charles Darwin University
Nano/mesoporous carbon from rice starch for voltammetric detection of ascorbic acid
Wahab, Mohammad A.; Darain, Farzana; Islam, Nazrul; Young, David James
Published in: Molecules
Document Version Publisher's PDF, also known as Version of record
Link to publication
Citation for published version (APA): Wahab, M. A., Darain, F., Islam, N., & Young, D. J. (2018). Nano/mesoporous carbon from rice starch for voltammetric detection of ascorbic acid. Molecules, 23(2), 1-11. . https://doi.org/10.3390/molecules23020234
General rights Copyright and moral rights for the publications made accessible in the public portal are retained by the authors and/or other copyright owners and it is a condition of accessing publications that users recognise and abide by the legal requirements associated with these rights.
• Users may download and print one copy of any publication from the public portal for the purpose of private study or research. • You may not further distribute the material or use it for any profit-making activity or commercial gain • You may freely distribute the URL identifying the publication in the public portal
Take down policy If you believe that this document breaches copyright please contact us providing details, and we will remove access to the work immediately and investigate your claim.
Download date: 27. Dec. 2020
https://doi.org/10.3390/molecules23020234 https://researchers.cdu.edu.au/en/publications/dcc97189-f28f-4361-8571-056003e967f6 https://doi.org/10.3390/molecules23020234
Nano/Mesoporous Carbon from Rice Starch for Voltammetric Detection of Ascorbic Acid
Mohammad A. Wahab 1,*,†, Farzana Darain 2,3,†, Nazrul Islam 4 and David James Young 1,* 1 Faculty of Science, Health, Education and Engineering, University of the Sunshine Coast, Maroochydore DC,
QLD 4558, Australia 2 Australian Institute for Bioengineering and Nanotechnology (AIBN), University of Queensland, St Lucia,
QLD 4072, Australia; email@example.com 3 Sugar Research Australia Ltd., Indooroopilly, QLD 4068, Australia 4 Pharmacy Discipline, Faculty of Health, School of Clinical Sciences, QUT, 2 George Street, Brisbane, QLD
4000, Australia; firstname.lastname@example.org * Correspondence: email@example.com or firstname.lastname@example.org (M.A.W.); email@example.com (D.J.Y.) † These authors contributed equally to this work.
Received: 7 December 2017; Accepted: 24 January 2018; Published: 25 January 2018
Abstract: Rice starch (RS-)based nano/mesoporous carbon (RSNMC) was prepared via a hard- templating route using cheap rice starch as a carbon source. XRD and TEM characterization indicated the formation of organized nanoporous RSNMC. Nitrogen absorption–desorption studies revealed a high surface area of up to 488 m2·g−1, uniform pore size of 3.92 nm, and pore volume of 1.14 cm3·g−1. A RSNMC-modified glassy carbon (GC) electrode was employed for the determination of ascorbic acid (AA) and exhibited a linear response in the concentration range of 0.005–6.0 mM with a detection limit of 0.003 mM. These results demonstrate that RSNMC has potential as an advanced and cheap electrode material for electrochemical sensing and other electrocatalytic applications.
Keywords: mesoporous carbon; carbon; rice starch; biomass; electroanalysis; ascorbic acid; electrode; glass carbon electrode; nanomaterials
Nano/mesoporous carbon materials (NMC) are of interest because of their high surface area, uniform pore structure, mechanical strength, chemical stability, and relative lack of reactivity [1–7]. These characteristics are suited to various applications including as electrodes and support materials, and for catalysis, adsorption, immobilization, energy storage, drug delivery, and electrochemistry [1–7]. The synthesis of NMC usually involves impregnation of a carbon precursor, commonly sucrose, polypyrole, or furfuryl alcohol, into the pores of mesoporous SBA15 silica in the presence of a catalyst, followed by carbonization at high temperature [1–7]. A catalytic chemical vapor deposition (CVD) method has also been reported for mesoporous carbon but requires specialized apparatus and harsh conditions .
In this context, sustainable nanoporous carbon materials from low-cost biomass have become an important area of investigation [5,6]. Recently, hollow carbon spheres for use in Li–S batteries have been produced using a sustainable approach involving the hydrothermal carbonization of monosaccharides as the carbon precursors and silica nanoparticles as the hard-templates . Similarly, carbon materials with lower porosity have been prepared for the same application by the carbonization of mixed colloidal silica and starch . Liu et al. have reported the generation of micro/mesoporous carbon from chemically modified banana peel for size-selective separation of proteins . It should be noted that carbon material from such biomass requires further chemical activation to create pores, which undoubtedly complicates the process.
Molecules 2018, 23, 234; doi:10.3390/molecules23020234 www.mdpi.com/journal/molecules
http://www.mdpi.com/journal/molecules http://www.mdpi.com http://dx.doi.org/10.3390/molecules23020234 http://www.mdpi.com/journal/molecules
Molecules 2018, 23, 234 2 of 11
In this study, we describe a sustainable and cost-effective one-pot synthesis of rice starch-derived nano/mesoporous carbon material (RSNMC) and its application as an electrode material for the detection of ascorbic acid (AA). Ascorbic acid (vitamin C) is an essential nutrient for living cells and plays an important role in metabolic and cell development processes [10–13]. It helps develop cells and heal injuries, ulcers, and burns, and is involved in the synthesis of collagen, blood vessels, cartilage, bones, and tendons [10–13]. It is also an active component in a variety of pharmaceutical dosage forms such as high potency multivitamin supplements for the prevention and treatment of vitamin C deficiency, common colds, mental illnesses, infertility, cancer and AIDS [10–13]. It is consumed as an antioxidant in a variety of pharmaceutical products, foods, fruits, vegetables, and soft drinks. Different methods have been developed for determination of AA in different matrices, including by titration, UV–vis spectrophotometry, capillary electrophoresis, fiber-optic reflectance spectroscopy, HPLC, thermogravimetry, fluorometry, etc. [13–29]. Electrochemical techniques offer advantages of simplicity, selectivity, stability, and applicability in different matrices. AA is electrooxidized on conventional electrode surfaces; however, this process occurs with high overpotential, which can cause fouling of the electrode surface by its oxidation intermediates or products [22,23]. Thus, these electrodes will have poor reproducibility and reduced selectivity and sensitivity. To overcome these problems, various materials have been immobilized on conventional electrode surfaces, including conducting polymers, ionic liquids, metal nanoparticles, carbon nanotubes, metal complexes, and polymeric films [24,25]. This study reports the use of cheap, nontoxic rice starch-derived nano/mesoporous carbon (RSNMC) as an electrode coating material for the detection of AA using cyclic voltammetry with a RSNMC-modified glassy carbon electrode.
2.1. Synthesis of the Hard Mesoporous SBA15 Silica Nano-Template
Surfactant Pluronic P123 (2.0 g) (Sigma-Aldrich, St. Louis, MO, USA) was added to 60 mL of 2 M HCl at 38 ◦C with vigorous stirring for 2 h. Tetraethylorthosilicate (TEOS) (4.2 g) (Sigma-Aldrich) was added dropwise to the surfactant-containing solution with stirring for another 8 min and left to stand for 24 h at 38 ◦C. This solution was then autoclaved at 100 ◦C for 24 h, filtered, and dried at room temperature. Finally, calcination was performed at 550 ◦C for 6 h in air [30–35].
2.1.1. Synthesis of Nano/Mesoporous Carbon (RSNMC) from Rice Starch
Rice starch (2.0 g) (Sigma-Aldrich) in 20 mL of deionized water was stirred in a beaker at 85–90 ◦C. SBA15 mesoporous silica template (2.3 g) (Figure 1a) was added slowly to the starch solution with vigorous stirring to ensure a homogenous solution of template and rice starch (Figure 1b). Stirring overnight yielded a viscous gel that was collected in a petri dish and dried in an oven at 60 ◦C for 12 h to remove the solvent, then at 100 ◦C for 6 h, followed by 160 ◦C for 6 h. Carbonization was carried out under an argon flow at 900 ◦C for 1 h The silica template was removed by washing with 5 wt % HF solution at room temperature for 6 h [30–35]. The resulting nano/mesoporous carbon (Figure 1c) was collected by filtration, washed with ethanol, and dried in an oven at 100 ◦C.
2.1.2. Electrode Preparation and Electrochemical Measurements
The RSNMC was predried at 60 ◦C for 1 h in a conventional oven. RSNMC (5 mg) was added to 20 mL of ethanol and sonicated for 30 min to obtain a well-dispersed, homogeneous suspension. The bare glassy carbon (GC) electrode was polished with 0.50 and 0.05 µm alumina slurry and rinsed with water. It was then sonicated in deionized water for 5 min and dried under a high-purity nitrogen stream. The RSNMC ethanol suspension (4 µL) was drop-cast onto the cleaned GC electrode and dried under a nitrogen atmosphere at room temperature to obtain the RSNMC/GC electrode.
Electrochemical experiments were performed on a Bioanalytical Systems BAS 100B/W electrochemical workstation with three e